OXIDATION BEHAVIOUR OF AUSTENITIC STAINLESS STEELS AT
HIGH TEMPERATURE IN SUPERCRITICAL PLANT
HENRY GEORGE SIMMS
A thesis submitted to
The University of Birmingham
For the degree of
MASTER OF RESEARCH
School of Metallurgy and Materials Engineering
College of Engineering and Physical Science
The University of Birmingham
University of Birmingham Research Archivee-theses repository
This unpublished thesis/dissertation is copyright of the author and/or third parties. The intellectual property rights of the author or third parties in respect of this work are as defined by The Copyright Designs and Patents Act 1988 or as modified by any successor legislation.
Any use made of information contained in this thesis/dissertation must be in accordance with that legislation and must be properly acknowledged. Further distribution or reproduction in any format is prohibited without the permission of the copyright holder.
Fossil power plant efficiency is improved by increasing steam temperature and pressure. Current martensitic and ferritic steels do not have the required oxidation and spallation properties for boiler tube applications as service conditions increase. Spallation inside the tube can lead to blockage, overheating, creep rupture and turbine erosion. The current steels are limited to 620oC, therefore austenitic stainless steels are proposed for boiler tube applications to enable higher operating conditions. This investigation compared the oxidation and spallation behaviour of the current martensitic steels (T91, T92) with the proposed austenitic stainless steels (super 304H, shot peened super 304H, 347HFG), in air at 600-700oC. Oxide morphology was characterised using SEM and EDX analysis and oxidation kinetics were recorded using specific mass gain and oxide thickness measurements over time. The martensitic steels formed non-protective Fe-rich oxides, which consistently spalled on cooling. The austenitic stainless steels showed little spallation and less mass gain compared to the T92 steel. Double-layered oxides formed on the super 304H and 347H FG steels consisting of an inner protective Cr-rich spinel oxide and an outer Fe-rich oxide. Shot peening increased the oxidation resistance of the super 304H steel forming significantly thinner, single-layer Cr-rich oxides with less mass gain.
1. Introduction 1
1.1. Industrial Practice for Power Generation – Steam Plants 1
1.2. Project Scope 3
2. Literature Review 4
2.1. Physical Metallurgy of Stainless Steels for Use in High Temperature Plants 4 2.1.1. The Effect of Alloying Additions on Microstructure and Properties
of Stainless Steel 4
126.96.36.199. Austenite Stabilisers 4
188.8.131.52. Solid Solution Strengthening 4
184.108.40.206. Creep Strength 5
220.127.116.11. Oxidation Resistance 6
18.104.22.168. Summary of Alloying Addition Functions 7
2.1.2. The Effect of Surface Modification on Physical Structure 8
22.214.171.124. Grain Refinement 8
126.96.36.199. Shot Peening 8
2.2. General Principles of Oxidation in Air 10
2.2.1. Principles of Oxidation 10
2.2.2. The Initial Stages of Oxidation 11
2.2.3. Oxide Transport Mechanisms 12
2.2.5. Oxidation of Alloys 17
2.2.6. Alloy Depletion 20
2.2.7. Scale Spallation 20
2.3. Oxidation in Water Vapour and Steam 23
3. Experimental Procedure 24
3.1. Materials 24
3.2. Isothermal Air Oxidation Tests 25
3.3. Sample Preparation and Cross Sectional Metallography 27
3.4. Oxide Thickness Measurements 28
3.5. Energy Dispersive X-Ray (EDX) Chemical Analysis 28
4. Results 30
4.1. Materials Characterisation 30
4.1.1. Composition 30
4.1.2. Grain Structure As-Received 33
4.2. Oxidation in Air 37
4.2.1. Mass Change Results 37
4.2.2. Overall Thickness Analysis 46
4.2.3. EDX Chemical Analysis 57
188.8.131.52. T91 Post Service 57
184.108.40.206. T92 60
220.127.116.11.2. T92 after Exposure 63
18.104.22.168. Super 304H after Exposure 68
22.214.171.124. Super 304H Shot Peened after Exposure 72
126.96.36.199. 347H FG after Exposure 77
5. Discussion 80
5.1. The Current Martensitic Steels used In Plant 80
5.1.1. T91 80
5.1.2. T92 81
5.2. The Proposed Austenitic Stainless Steels 83
5.2.1. Super 304H 83
5.2.2. Shot Peened Super 304H 87
5.2.3. 347H FG 88
6. Conclusions and Further Work 90
6.1. Conclusions 90
6.1.1. The Martensitic Steels 90
6.1.2. The Austenitic Stainless Steels 90
6.2. Further Work 91
A. Appendix 93
A.1. Oxidation in Water Vapour and Steam 93
A.1.1.1. The Dissociation Mechanism 94
A.1.1.2. Oxidant-gas Penetration Mechanism 96
A.1.1.3. Formation and Volatilisation of Fe(OH)2 96 A.1.1.4. Formation and Volatilisation of CrO2(OH)2 97 A.1.1.5. Proton Dissolution Induced Changes in the
Oxide Defect Structure 98
A.1.2. Steam Oxidation as a Function of Steel Composition and
Alloy Type 99
A.1.2.1. Ferritic Steels 99
A.1.2.2. Martensitic Steels 100
A.1.2.3. Austenitic Steels 101
A.2. Oxide Thickness Measurements 102
1.1. Industrial Practice for Power Generation – Steam Plants
Unlike other fossil fuels, there are no imminent dangers of running out of coal and it will remain a vital workhorse for energy generation well beyond the first half of the 21st century. In the UK 74% of the electricity demand is met by fossil-fuelled plants (38% coal- or oil-fired and 36% gas-fired) . Of the gas-fired plants half are combined cycle (i.e., gas turbine + steam turbine), therefore making >50% of UK electricity generation dependent on steam plant . The efficiency of conventional fossil power plants is a strong function of increased steam parameters (i.e., temperature and pressure), with the steam referred to as supercritical when reaching temperatures of 538-565oC and exceeding pressures of 22MPa in the main steam line. Increasing the temperature and pressure in a steam turbine increases the efficiency of the Rankine steam cycle used in power generation. Current state-of-the-art plants in the UK operating at a steam temperature of 565°C and a steam pressure of 17 MPa have a thermal efficiency of approximately 35%. An increase in plant efficiency from 35% to 50% is estimated to decrease CO2 emissions by 30% . This can be achieved by increasing the service conditions to pressures of 30 MPa and temperatures up to 600-650ºC . Other countries are already starting to build higher efficiency coal plants operating at 600-620oC. Considering the thousands of coal-fired power plants that India and China will build in the coming decades (e.g., China, in 2006 alone, built more electric power plants than the total installed capacity of Great Britain), the global impact that may occur when conventional power plants become nearly twice as efficient is substantial, perhaps cutting green house emissions to levels needed to offset the higher consumption of fuel.
Increasing the efficiency to 60% using ultra-supercritical steam (above 565oC and 27.5MPa in the main steam line) requires a significant increase in operating temperatures and pressures. Long-term research programmes such as USC in the US and THERMIE in Europe target 800°C and 35-39 MPa operating conditions . These operating conditions require new materials that can withstand these extreme temperature and pressure environments. Current ferritic and martensitic steels do not have the required mechanical properties at these temperatures, particularly creep rupture strength and thermal fatigue . Although materials
for these applications are primarily designed on creep properties, oxidation and spallation are key performance parameters in boiler tube applications due to temperature and pressure increases in service conditions that are already extremely harsh. Boiler tube steels have three main requirements; a need for tolerance to all stages of the fabrication process including welding, a need for adequate creep strength, and a need for sufficient fireside corrosion and steam side oxidation resistance . Spallation of a formed steam side oxide can have severe adverse effects such as collection of the spalled material in the bottom of tube bends, leading to blockage, overheating and premature creep rupture as well as transportation of the oxide through the system to the main steam valves and turbine, resulting in erosion damage [7, 8]. Fast scale formation can also lead to the consumption of the steel walls until the load bearing section is reduced and mechanical failure occurs . The main cause of oxide spallation is due to the stresses induced by a temperature drop. This drop in temperature can be due to intermittent service or thermal cycling of the tubes. To reduce the impact of spallation at higher service temperatures these plants should be used for continuous service. Where cyclic service conditions are expected lower peak service temperatures should be used . The mechanism responsible is the build up of internal stresses in the oxide layer due to a difference in thermal expansion coefficients between the different oxide layers and the substrate. However, creep can partly relax these stresses if the cooling rate is low enough .
Although improvements continue due to alloying additions, currently available ferritic and martensitic steels will be limited to use at temperatures up to 620°C. The oxidation and hot corrosion behaviour of these alloys in steam limit their temperature of operation as there are no obvious routes for improvement that will not invalidate the compositional restrictions set by the strengthening requirements . Improved understanding of the oxidation and spallation mechanisms in steam is necessary for lifing and progressive degradation assessment of existing materials as well as for future alloy design.
Austenitic steels are currently being used in the highest temperature regions of superheaters and reheaters in conventional stations. There has been a history of spallation events in martensitic steels over many years leading to tube failures. Stations recently built in China operating at higher steam temperatures  have reported oxide spallation and tube blockages. With increasing service temperatures (600oC and upwards) more austenitic stainless steel
tubing will be used in superheater and reheaters and more emphasis will be placed on the need for oxidation/corrosion resistance over increased mechanical strength. These higher chromium stainless steels will enable higher operating temperatures beyond the ferritic/martensitic steels’ limit, thus allowing the plant to work at higher steam parameters, leading to increased efficiency.
1.2. Project Scope
In this project the oxidation resistance of two candidate austenitic stainless steels (i.e., 304H and 347HFG) will be tested extensively in laboratory air conditions at a temperature range of 600-700oC. Results will subsequently be compared to the previous ferritic/martensitic steels (i.e., T91, T92) that are currently in use.
Therefore the main aims for this project are to;
1) Test the oxidation resistance of selected austenitic alloys in air by recording oxide growth and the spallation activity during and after high temperature exposure.
2) Record the oxide morphology using cross section analysis involving SEM and EDX testing.
3) Record the oxidation kinetics using mass gain and oxide thickness measurements over selected durations.
2. Literature Review
2.1. Physical Metallurgy of Stainless Steels for Use in High Temperature Plants
2.1.1. The Effect of Alloying Additions on Microstructure and Properties of Stainless Steel
The key materials properties for boiler tubes in power generation are high temperature strength and good corrosion resistance. Optimisation of these properties ensures that these steel components do not fail under working conditions. Although the use of steels is very common in boiler tube applications, additions of varying amounts of different alloying elements provide a range of these required properties in the extreme environments of the application.
188.8.131.52. Austenite Stabilisers
Nickel and manganese are added to steels to stabilise the face centred cubic austenitic structure and they guarantee complete austenitic formation during the austenisation treatment [12, 13]. The addition of chromium alone to a plain carbon steel causes ferrite to form . It should be noted that nickel also accelerates the coarsening of the precipitates causing the long term creep strength to decrease. Manganese is not as strong as nickel at stabilising the austenite but it has the same effect on coarsening of the carbides and reducing the creep strength. They both have a strong solid solution strengthening effect in iron as well . Copper also has an austenitic stabilising effect although its main purpose in the alloy is to improve the creep strength . In type 347H FG the structure is also stabilised by tantalum and niobium additions for service at high temperatures . This austenitic structure is important as these steels are readily fabricated and unlike ferritic steels, they do not undergo the undesirable ductile/brittle transition .
184.108.40.206. Solid Solution Strengthening
Nitrogen is added to the stainless steel to increase the tensile strength of the alloy through solid solution strengthening. In service the nitrides can precipitate, which reduces dissolved
nitrogen in the austenitic matrix decreasing the solid solution strengthening . While the formation of nitrides and carbides during service is beneficial for creep resistance, niobium carbonitride phases also precipitate during service helping to strengthen the alloy. Niobium is also a strong and stable carbide and nitride former. Un-dissolved niobium carbides are often wanted as they restrict grain growth during austenisation of the alloy which is desirable for reasons discussed later . For these to dissolve completely they have to be heated above austenising temperatures . Some carbides form on grain boundaries increasing the boundary strength . The formation of chromium carbides causes a depletion of chromium in the matrix reducing the oxidation resistance [13, 15]. In austenitic steels, carbon and nitrogen have high solubility and act as strong austenite stabilisers . Carbon is also added for its solid solution strengthening effect to restrict the movement of dislocations in the metal . Phosphorus is also involved in increasing the hardenability. It segregates to the carbide surface or is integrated in them which slows down the coarsening rate of the carbide stabilising the microstructure .
220.127.116.11. Creep Strength
Type 304H austenitic stainless steel is used in conventional power plant where metal temperatures are below 600oC. However, creep resistance of standard 304H is not good enough for temperatures above 600oC in power generation applications. Therefore, copper and other alloying additions of up to 3 wt% are included in the composition to improve the creep strength [13, 14]. This new alloy design is called ‘super 304H’ and its improved creep strength is also due to increased carbon content and certain amounts of niobium and nitrogen which are added. An alternative method of increasing the creep strength is increasing the nickel content, but this also increases the cost of the alloy considerably and so is not desirable . Copper improves the creep strength by the precipitation of the copper rich phase in the matrix during service reducing the motion of dislocations via precipitation hardening. The precipitation of this phase is accompanied by the precipitation of a niobium carbonitride phase . During long term service of the steel, the copper rich precipitates coarsen which means their strengthening effect is reduced. The copper rich precipitates have a critical diameter of around 30 nm after which they are no longer coherent with the austenitic matrix and the creep strengthening is less effective. So the aim is to avoid this effect in service and from this an optimum copper addition of 3 wt% is achieved . Type 347H FG is stabilised with niobium
which can be heat treated to produce NbC carbides which improve creep strength by interacting with dislocations produced throughout creep . Type 304H and 347H FG also contain carbon contents higher than 0.04wt% which enable elevated and reproducible creep rupture strength at high temperatures .
18.104.22.168. Oxidation Resistance
The chromium content in the alloy is extremely important for improving the oxidation/corrosion resistance of the steam side of the pipe [13-15, 17], by the formation of a protective, adherent, slow growing Cr2O3 (chromia) oxide layer . This oxide is slow growing and blocks the outward diffusion of other alloy elements and the inward diffusion of gaseous impurities  as transport processes through this scale are generally slow . The outward diffusion of chromium (Cr3+) along grain boundaries has shown to be faster than the inward diffusion of oxygen by a factor of three and so the chromia scale usually grows outward  and can contain small amounts of iron, nickel and manganese  as seen on high chromium steels such as 310. Chromium content is important in dictating the oxide formed, lower chromium concentrations e.g. type 304, form the spinel oxide FeCr2O4 which can be protective to a lesser extent . The greater the chromium content in the alloy the greater its oxidation resistance is . Steels with a chromium content of over 13 wt% show very low oxidation rates and their scales consist of Cr2O3, (Cr, Fe)2O3 or Cr rich (Cr, Fe Mn)3O4 with an outer layer of Fe2O3 . However, at temperatures exceeding 900oC, chromia scales can react further with oxygen to form CrO3 which is a volatile species .
Silicon additions are also well known for enhancing the oxidation resistance of stainless steels with the lower silicon concentrations having the highest corrosion rates [9, 15, 21, 22]. This effect has been explained by suggestions such as the formation of the initial chromia layer being facilitated by silicon, or the formation of silica particles beneath the chromia layer which increase the adhesion of the chromia layer, or the formation of a continuous silica layer beneath the chromia preventing outward diffusion of chromium ions . The additions of both chromium and silicon at optimum levels will improve oxidation resistance without adversely affecting the creep strength . The influence of silicon is enhanced at higher temperatures, i.e. above 700°C .
Manganese is also an alloying addition seen to affect oxidation resistance, but its effect has been measured both favourably and adversely [15, 23]. In some cases it has been found to be damaging to the oxidation resistance of austenitic stainless steels due to it forming a spinel oxide of MnO·Cr2O3 rather than the protective chromia oxide . Nickel has also been shown to enhance the oxidation resistance by reducing the cation diffusion in the Cr2O3 scale and preventing the formation of FeCr2O4 + Fe2O3, having an influence on the adhesion and mechanical properties of the scale . It is very difficult to consider these alloying elements separately due to their complex interactions.
22.214.171.124. Summary of Alloying Addition Functions
The various alloying additions and their role in steel is summarised in table 2.1. All of the alloying elements are added to optimise the steel’s properties so that they do not fail in service.
Table 2.1. Review of alloying addition functions.
Alloying Element Function
Nickel Stabilises the austenitic structure during the austenisation treatment. Manganese Stabilises the austenitic structure during the austenisation treatment.
Nitrogen Increases the tensile strength through solid solution strengthening.
Niobium Stabilises carbon and improves the creep strength by forming NbC carbides. Carbon Increases the tensile strength through solid solution strengthening.
Copper Improves the creep strength by the precipitation of a copper rich phase. Also has an austenitic stabilising effect.
Chromium Improves the oxidation/corrosion resistance. Resistance increases with increasing chromium content.
Silicon Improves the oxidation/corrosion resistance. Phosphorus Involved in increasing hardenability and strength.
2.1.2. The Effect of Surface Modification on Physical Structure
126.96.36.199. Grain Refinement
The grain size also influences the oxidation resistance of the alloy. Short circuit diffusion of ions along the grain boundaries is a lot quicker than through the grains themselves [14, 16, 19, 24-26]. Reducing the grain size increases the grain boundary density which in turn increases the rate at which chromium ions can diffuse through the alloy . This leads to the early formation of the Cr2O3 oxide layer, slowing down further growth of the oxide layer due to its low permeability  . A study on 304 stainless steel in wet air revealed catastrophic breakaway oxidation on coarse grained samples due to the formation of a non-protective iron-rich scale; samples with fine grain structure did not show breakaway oxidation due to the dense network of grain boundaries increasing the chromium diffusion which promoted stable growth of the protective chromium-rich scale . A study in laboratory air of TP347 showed a similar grain size effect; Cr2O3 formed on the fine grained variant but the coarse grained equivalent formed non-protective iron based oxides . Grain refinement is an alternative method to adjusting alloy composition to help protect against oxidation  and also increases the strength by impeding the motion of dislocations .
188.8.131.52. Shot Peening
Another technique used to increase the oxidation resistance of the stainless steels is a surface modification technique called shot peening [9, 14]. This method involves inducing compressive stresses in the surface via impact of peening beads . This treatment causes the grain boundary density and twin boundaries near the surface (~50µm) to increase through cold deformation . The grains are refined via dislocations from sub-micron to nano-sized grains . As with the grain refinement method, this increases the chromium diffusion to the surface to produce a protective Cr2O3 oxide scale [9, 14, 29]. A study by Tan et al. in 2008  also showed the shot peening treatment to improve oxidation resistance. In this study alloy 800H displayed improved oxidation resistance in supercritical water after shot peening. This was due to the shot peened surface having a deformed surface zone consisting of two microstructural regions; an ultra fine grained region at the surface and a transition region at the sub surface . The shot peened samples had thinner oxide scales that mainly consisted of
chromia due to the enhanced chromium diffusion and less scale exfoliation was seen compared to the samples with no surface treatment . Shot peening not only increases oxidation resistance but also increases fatigue life, hardness/durability, closing of porosity and stress corrosion cracking resistance .
2.2. General Principles of Oxidation in Air
2.2.1. Principles of Oxidation
The general chemical equation for an oxidation reaction between a metal (Me) and oxygen (O2) is shown below.
aMe + b/2 O2→ MeaOb (Eq. 2.1)
It is a simple equation but it depends on several factors and can become more intricate .
The first step in this metal-oxygen reaction involves the adsorption of gas on the clean metal surface. The adsorbed oxygen dissolves into the metal and the oxide forms as separate oxide nuclei or as a continuous oxide film. The solid reaction product (metal oxide) separates the two reactants, and for the reaction to continue further, one or both reactants have to penetrate the oxide layer (scale) by solid-state diffusion. This can happen by either oxygen going through to the oxide-metal interface and reacting there, or the metal being transported through the oxide to the oxide-gas interface and reacting there as shown in Figure 2.1 . For thick compact scales, the reason for transport through the oxide is due to the chemical potential gradient across the scale, and for thin films it may be due to electric fields across the film. In porous oxides solid-state diffusion is limited and can be restricted to diffusion occurring at phase boundaries, or mass transport occurs through gas diffusion. Oxide layers at very high temperatures can also be volatile or liquid .
Figure 2.1. Schematic showing a simplified diffusion controlled process of oxidation where the cations and cation vacancies have to penetrate the oxide scale for the reaction to continue .
2.2.2. The Initial Stages of Oxidation
The adsorption of gas onto the metal surface is the very first stage of oxidation. This process involves a decrease in free energy and entropy which means enthalpy decreases and makes this process normally exothermic. There are two types of adsorption, chemical (chemisorption) and physical. Chemisorption involves the adsorbed species forming a chemical bond with surface atoms via the transfer of electrons. Physical adsorption involves physical or van der Waals forces bonding the gases to the surface and is reversible . Chemisorption tends to take place at much higher temperatures and may involve an activation energy. Very rapid chemisorption can be seen with gases and clean metals where there appears to be no activation energy. It continues only until a monolayer of the adsorbent is created on the surface .
After the adsorption where the surface has been covered by chemisorbed oxygen, isolated oxide nuclei nucleate at random points for instance at impurity atoms, surface imperfections etc. on the metal surface. The growth of individual crystallites enables the oxidation of the surface to continue until oxide patches grown from individual nuclei connect and the entire surface is covered with oxide which acts as a diffusion barrier [17, 30].
2.2.3. Oxide Transport Mechanisms
The formed oxide separates the metal from the gas and the only way for oxidation to proceed is via solid-state diffusion of the reactants. This type of diffusion can only take place due to the presence of defects in the oxide structure. Point defects such as vacancies, interstitial atoms and misplaced atoms are required for solid-state diffusion in the oxide [17, 30]. Scale growth occurs by the diffusion of the cations and anions. Cation diffusion causes oxide formation at the oxide-gas interface and anion diffusion leads to oxide growth at the metal-oxide interface as shown in Figure 2.2. Oxides can show nonstoichiometry and either mainly contain cation defects or mainly contain oxygen defects.
Figure 2.2. Schematic of high temperature oxidation mechanisms, showing the reactions at the metal interface and transport routes of ions where the cation is mobile (a) and the anion is mobile (b) .
2.2.4. Reaction Kinetics
The rate of oxidation can be measured experimentally by using three methods. These involve measuring the amount of oxygen consumed, the amount of metal consumed or the amount of oxide produced. The method used to find the amount of metal consumed is the least preferable as it is a destructive method which is indirect and not continuous. The method chosen in this project is to record the amount of oxide produced by weight change measurements and oxide thickness measurement. All of these variables are measured as a function of time to show the
rate of oxidation . From experimental data three main rate laws have been observed as follows;
1.) The linear law: this is where the rate of reaction is constant with time and independent of the quantity of metal or gas consumed up to that time. The initial surface reaction step (adsorption) or the diffusion through the gas phase controls the oxidation process and is said to be rate determining. The linear rate law can be observed at the very initial stages of oxidation when the metal surface is exposed to the atmosphere for the first time. It can be described by the following equation,
x = klt (Eq. 2.2)
where x is the scale thickness, kl represents the linear rate constant and t is the time .
2.) The parabolic law: this is where the rate of reaction is inversely proportional to the square root of time . Many metals at high temperatures show this rate law where the diffusion of ions, either metal or gas, through the compact scale is the rate determining process . The parabolic law can be described by the following equation,
x2 = 2k′t (Eq. 2.3)
where k′ is the scaling constant . These two laws can be displayed graphically so the oxidation kinetics can be observed easily as shown in Figure 2.3.
Figure 2.3. A graph showing linear and parabolic oxidation where oxide growth (x) is a function of time (t) .
3.) The logarithmic law: this is characteristic of the oxidation of a lot of metals at low temperatures (usually below 300-400oC) and for the formation of very thin oxide films below tens of nm thick . The reaction starts off rapidly and then slows down as it proceeds, this rate law can be described by two equations,
Direct logarithmic: x = klog log (t + t0) + A (Eq. 2.4)
Inverse logarithmic: 1/x = B - killog t (Eq. 2.5)
where klog and kil are rate constants and A and B are constants . These laws can also be shown graphically as seen in Figure 2.4.
Figure 2.4. A graph showing the logarithmic and inverse logarithmic oxidation kinetics where oxide growth (x) is a function of time (t) .
Oxidation reactions often tend to follow a mixture of different rate laws as described above. This is due to the rate determining mechanisms changing during the reaction due to the scale itself changing or the reaction having concurrent mechanisms and one dominating at the start and then the other mechanism taking over later on . An example of this is the transition from linear to parabolic law. The reaction starts off at constant rate when the oxide is just forming and is thin so diffusion through the film is very fast. Here the surface reaction is the rate determining mechanism. As oxidation continues and the scale becomes thicker there is less ion flux through the scale and the reaction rate decreases. The diffusion of ions through the oxide is now the rate determining step and the rate decreases as the reaction proceeds displaying the parabolic law .
The parabolic relationship is the most desirable as the oxide formed is slow growing and less likely to spall. This relationship is shown by curve OAD in Figure 2.5. However, depending on conditions (alloy composition, time and environment) breakaway oxidation can occur where there is a sudden increase in the growth rate shown by curve AB . In the case of stainless steels, this is where iron rich oxides are forming instead of chromia due to alloy depletion as discussed later. The growth of oxide can continue shown by curve BE, possibly due to the environment where volatilisation of the oxide occurs, or from cracking in the scale
leading to additional outbursts of quick oxidation . Alternatively, the oxidation rate can decrease again, BC, if a protective oxide reforms.
2.2.5. Oxidation of Alloys
All of the principles that have been described previously have been for simple oxidation of pure metals but this theory can also be applied to alloys. However, the oxidation of alloys can be a lot more complex due to the metals in the alloy having differing affinities to oxygen because of the different free energies of formation of the oxides. The different metals will also have varying diffusivities in the alloy and their ions will have different mobilities in the oxide phases . This makes the prediction of oxidation behaviour much more difficult for alloys.
To have effective oxidation resistance the alloy needs to form a continuous scale via external oxidation. Ineffective protection can occur by precipitates forming inside the alloy during oxidation, this is called internal oxidation . To achieve effective oxidation resistance, alloys aim to form compact scales with small rates of diffusion of the reactant ions .
The oxidation of alloys generally produces more than one oxide. Selective oxidation occurs where the least noble alloying element in the alloy is oxidised first to form the outer protective layer . The alloying elementshaveoxides which demonstrate large differences in stability; however, the temperature, partial pressure of the oxygen and concentration of the active alloying element also affect selective oxidation . Selective oxidation has lead to alloys being designed to have certain alloying additions in them to increase their oxidation resistance in high temperature applications. However, adding elements that help form protective oxide scalestends to have a negative effect on other alloy properties such as mechanical properties, and so these element additions need to be as low as viably possible . Chromium, aluminium and silicon are the three main elements that when added constantly form protective scales. Their oxides have the lowest diffusion rates making them the optimum protective oxides . For most industrial high temperature alloys, the base metal consists of iron, nickel or cobalt which all form moderately stable oxides, and additional alloying elements such as chromium, aluminium and silicon which form highly stable oxides . Silicon additions have been found to reduce the weldability and toughness of steels and nickel based alloys, and so its concentration has to be limited to reduced levels where the formation of silica alone cannot be attained .
Iron-chromium alloys are a very common commercial alloy for high temperature applications. When there are small concentrations of chromium in the alloy both iron and chromium rich oxides form on the surface. The chromium solubility in the FeO phase is limited and so only some chromium will enter this phase . If the chromium content is increased in the alloy the Fe2+ ions are blocked by the FeCr2O4 islands so the FeO layer gets thinner compared to the Fe3O4 layer. At a low concentration of chromium the reaction rate is still quite low . If the chromium content is further increased then the parabolic rate constant is lowered due to a mixed spinel of Fe(Fe,Cr)2O4 forming. Iron ions appear to be more mobile than chromium ions in this oxide because at longer durations pure iron oxides are formed on the outer surfaces of the scale . When the chromium content increases to a critical concentration the scale formed initially is Cr2O3 which reduces the parabolic constant further. This protective scale can only be formed at chromium concentrations which surpass this point. This is taken into consideration when designing heat resistant alloys such as stainless steels .
When designing the alloy and its composition for oxidation resistance the Ellingham diagram can be very helpful as it displays and compares the stability of the possible oxides forming under stated conditions. This helps show which elements in the alloy will oxidise preferentially over the others and which will oxidise next when the initial element becomes depleted. The Ellingham diagram shown in Figure 2.6 has different lines for different oxidation reactions. The lines represent the standard free energy of oxidation of pure metals versus time . The lower the line on the diagram, the more stable the oxide formed is and the lower its dissociation partial pressure . Chromium, silicon and aluminium are all low down in the diagram, below the iron oxides, and they are all capable of forming stable protective oxides when present in the right concentrations in the alloys.
2.2.6. Alloy Depletion
As the oxidation reaction occurs at high temperature the oxide formation needs to be provided with a supply of the active elements from the substrate. If the active element is not in the adjacent area to the oxide then this will become the rate determining factor. The active element is consumed in the substrate during the reaction via diffusion towards the oxide. The region of substrate beneath the oxide layer then becomes depleted of this active element. Further depletion could lead to the protective oxide being unable to be maintained due to concentration of the active element becoming too low. This can lead to breakaway oxidation [34, 35].
The chromium depletion zone can have a positive effect on spallation resistance as this de-alloying can change the microstructure and therefore mechanical properties. If the depleted zone is weaker than the substrate then creep will occur here and reduce stresses built up from thermal cycling and thermal expansion coefficient mismatches. These relaxed stresses help prevent spallation .
2.2.7. Scale Spallation
The scales formed from the oxidation reaction usually experience mechanical stress which is what causes fracture, microcracking, scale delamination and spallation. When the stress in the scale increases to the limit accommodated by elastic strain, it will deform or fracture . The spallation of the scale removes its protective function allowing direct access of the environment to the metal beneath and leads to a rapid increase in oxidation [36, 37]. Therefore it is desirable to design and use alloys that form oxides which do not fracture and spall . Repeated spallation in alloys with a low chromium concentration can lead to alloy depletion where the protective chromia oxide will no longer form . The stresses in the oxide are influenced by the stresses changing in both the metal and the oxide. These stresses can grow during oxidation itself, called growth stresses1 where the specific volume of the oxide is
1 Growth stresses can be caused when the volume changes caused by oxidation can be inhibited by the shape of
the alloy or structure, which can cause the oxide to incur strain or start to deform. This is due to the fact that the specific volume of the oxide is usually not the same as the volume of the metal being consumed in the reaction
usually not the same as the volume of the metal being consumed in the reaction, which can also be influenced by specimen geometry; see Figure 2.7 [18, 31, 38]. Concurrent radial stresses also grow in the oxide as seen in Figure 2.7. Compositional changes due to depleted elements as discussed in the alloy depletion section can also cause growth stresses in the scale but also relieve stress by creep. Generally any deformation to the substrate material will be transferred to the adherent oxide .
Figure 2.7. The effects of specimen geometry on scale growth stresses with the dark grey shading signifying newly grown oxide .
. The specimen geometry is highly influential on growth stresses as additional stresses can occur during oxidation of curved metal surfaces such as tubing. The type of stresses that arise will depend on the type of curvature and the mechanism of scale growth . There are four different scenarios shown in Figure 2.7 that could occur when the common condition where the volume of oxide/volume of metal > 1 exists: convex surfaces experiencing anionic oxidation, convex surfaces experiencing cationic oxidation, concave surfaces experiencing anionic oxidation and concave surfaces experiencing cationic oxidation [31, 38]. For the convex surface experiencing oxygen diffusion (anionic), the metal-oxide interface recedes and the oxide is compressed tangentially into the smaller volume where the metal was previously .
The second type of stresses that arise in the oxide layer are thermal stresses caused by differential thermal expansion or contraction in the oxide and the substrate during temperature change . The extent of thermally induced stresses is dependent on the size of the temperature change and the difference in thermal expansion coefficients of the oxide and the substrate. These usually put the scale formed under compressive stress on cooling causing fracture and spallation . Thus, cyclic exposure tends to be harsher than isothermal exposures [19, 31]. The following equation  expresses the magnitude of these thermal stresses when the alloy cools from temperature T1 to temperature T2;
where E = elastic modulus, δ = thermal expansion coefficient, y = thickness, and c, m = subscripts referring to oxide and metal respectively.
If δm > δc then the stresses are compressive and quickly induced leading to scale failure .
The component or specimen responds to these stresses by either the oxide cracking or spalling from the substrate exposing fresh metal to the oxidising gas, or by plastic deformation of the substrate or the oxide . Oxide cracking occurs when it is under tension, but most oxides are under compression due to the growth and thermal stresses being compressive. Spallation due to compressive stresses can occur by either buckling or wedging shown in Figure 2.8 . This will depend on factors such as scale thickness, defect size in the oxide and the fracture toughness of the scale or scale/metal interface . Wedge cracking occurs when the scale is less resistant to rupture than the substrate-scale interface. Compressive shear cracks form in the scale first then decohesion at the interface occurs . Buckling occurs when decohesion occurs first at the interface without through thickness cracking of the scale. The compressive stresses causes the scale to buckle during cooling until finally tensile cracks propagate at the points of greatest curvature in the scale to relax the stress and strain .
Figure 2.8. Schematic representation of oxide under compression fracturing via wedging (Route 1) and buckling (Route 2) .
2.3. Oxidation in Water Vapour and Steam
For a detailed description of the oxidation of steels in water vapour and steam, and the associated mechanisms, see Appendix 1.
3. Experimental Procedure
The materials studied in this project were a selection of four steels ranging from materials that are currently in use in plant (i.e., martensitic steels), and the proposed new materials which are the ‘18/8’ austenitic (300 series) stainless steels with higher chromium content. In addition, a variant on the super 304H was also tested; these specimens had a shot peened inner bore. All of the steels were received in tube form as they would go into the RWE Npower plant. These steels designations and composition in weight percentage are shown in the Table 3.1.
Table 3.1. Steel Composition in wt% (white) and at% (grey).
C Si Mn P S Ni Cr Mo W Cu V Nb Al B N 0.11 0.31 0.46 0.015 0.0038 0.09 9.46 0.88 - - 0.2 - - - - T91 0.51 0.55 0.46 0.03 0.0065 0.08 9.98 0.51 - - 0.22 - - - - 0.098 0.29 0.42 0.007 0.0013 0.13 9.5 0.36 1.74 - 0.19 0.062 0.009 0.002 0.0462 T92 0.46 0.55 0.43 0.01 0.0022 0.12 10.06 0.21 0.53 - 0.21 0.04 0.02 0.01 0.18 0.1 0.2 0.8 - - 9 18 - - 3 - 0.4 - - 0.1 Super 304H 0.46 0.39 0.84 - - 8.29 19.35 - - 2.60 - 0.24 - - 0.39 0.08 0.75 2 0.04 0.03 11 18 - - - - 0.82 - - - 347H FG 0.36 1.64 2.18 0.07 0.05 10.38 19.13 - - - - 0.48 - - -
All steel tubes were supplied in the as-received condition, i.e. as they go into plant, except for the T91 which was a post-service sample that had been exposed to steam at temperatures of 580oC ±20oC for a duration of approximately 79000 hours. This tube was studied solely for morphological comparison. The T91 and T92 tubes are both martensitic and are currently used in plant. The super 304H and 347H FG are both austenitic stainless steels and are being proposed for future plant use at higher steam parameters. It should be noted that the chromium concentration of these austenitic stainless steels are similar. The dimensions of the tubes received from RWE Npower are shown in Table 3.2.
Table 3.2. Tube dimensions.
Steel Outside Diameter / mm Wall Thickness / mm
Super 304H shot peened 41.3 6.5
Super 304H 42.4 5.6
347H FG 38.1 4.5
T92 51.5 8.0
T91 post service 53.0 8.9
The tubes were sectioned into rings approximately 25mm in length. These were further sectioned into six radial sections producing specimens, as shown in Figure 3.1, for examination and oxidation testing. Cut edges were removed/smoothed using 1200 grit SiC paper with a water lubricant. One specimen from each batch was examined in the as-received condition.
3.2. Isothermal Air Oxidation Tests
The inner surfaces of all the specimens were tested in their as-received condition except T92. The T92 specimens were found to retain some residual oxide on the inner surface in the as-received condition. To assess its affect, half of this surface was abraded with a series of silicon carbide papers; 240, 400, 800 and finishing with 1200 grit paper. The other half of the inner surface was left in the as-received condition with the original oxide layer as shown in Figure 3.1. Each sample was weighed using a highly sensitive electronic scale, accurate to ±0.000005g. The dimensions of each sample were measured and recorded using a digital micrometer so that the surface area of each specimen could be calculated. Finally, each sample was cleaned just prior entering the furnace in an ultrasonic bath with acetone.
Figure 3.1. T92 sample with half the inner surface abraded to 1200 grit (right side) as it would go into the furnace.
The samples were tested in batches of four, one from each tube, with their inner surfaces facing uppermost. The furnaces used were Elite Thermal Systems Ltd tube furnaces (Figure 3.2) which were calibrated using and an external calibrated thermocouple and voltmeter. In each case the size of the heat zone was confirmed by taking calibrated temperature readings along the furnace tube. The furnace was set to the required temperature before inserting the samples. The tests were conducted at 600oC, 650oC and 700oC in laboratory air for 100h, 250h, 500h and 1000h. On completion the specimens were removed and left to cool in laboratory air. Once cooled, the samples were re-weighed and the mass change per unit surface area was calculated without including the spalled oxide mass.
Samples were visually inspected for signs of gross spallation. Images were taken with an Axiovision Macroscope of the inside surface of each sample to record the oxide surface appearance. The inner surface of each tube, in the as-received condition, was also examined using Scanning Electron Microscopy.
3.3. Sample Preparation and Cross Sectional Metallography
The samples were prepared for cross-sectional analysis using standard techniques. To prevent damage to the oxide scale the oxidised samples were vacuum impregnated with a low viscosity Epofix resin. Once the resin had cured the sample was transversely sectioned at the mid length using a silicon carbide cutting disc and an especially slow feed rate of 0.015mm/s to prevent damage to the oxide scale. The sectioned sample was then mounted in a Tri Hard resin to aid the polishing process. The samples were manually ground under tap water using successive silicon carbide paper of 120, 240, 400, 800 and then 1200 grit. All samples were cleaned between stages with tap water and degreaser, with a further clean in ethanol and fan dried before the polishing stage. The samples were manually polished to 6µm using a Mol cloth and 6µm diamond suspension, followed by polishing using a Nap cloth and 1µm diamond suspension. The final polish was performed on an automatic Syton Polisher using OP-S colloidal silica suspension which provides a 0.04µm finish. The same cleaning process was also used between all of the polishing stages.
To observe the different grain structures of the steels, selected samples were etched and examined using optical microscopy. The martensitic steel (T92) was etched by swabbing the sample in Viella’s solution for 5 seconds. The austenitic steels were etched electrolytically in 10% oxalic acid for 30 seconds each. Digital optical microscopy of up to 100x magnification was used to observe and record the microstructure of each steel.
For examination using Scanning Electron Microscopy (SEM) and Energy Dispersive Spectroscopy (EDS) the samples were sputtered with gold to produce an electrically conductive layer, and subsequently painted with silver to increase the conductivity further and reduce charge build up in the scanning electron microscope (SEM).
The Jeol 6060 tungsten filament and Philips XL 30 LaB6 SEM were used to take micrographs of inner surface region of each sample at different magnifications along the whole oxide to get representative images. All SEM work was performed using a 20 keV accelerating voltage throughout. Back scattered electron images were preferred over secondary electron images as the oxide was more visible and composition changes could be observed.
3.4. Oxide Thickness Measurements
For each image a scale calibration was made, and ten equidistant oxide thickness measurements were made using ImageJ software (Figure 3.3). The specimen surfaces were rarely flat and so measurements were made perpendicular to the substrate surface, i.e. the growing direction. This produced 60 oxide thickness measurements for each sample so that the mean and standard deviation could be gained for a thorough assessment of thermally grown oxide (TGO) thickness.
Figure 3.3. A SEM image showing an example of where the oxide thickness measurements would be made using ImageJ, depicted by the red pointers.
3.5. Energy Dispersive X-Ray (EDX) Chemical Analysis
Chemical analysis of the sample cross section was performed using Oxford Instruments energy dispersive X-ray spectroscopy (EDX) with the INCA software. Several point scans were made along the oxide layer/layers and averages calculated to help identify the different
oxide layers forming. Line scan analysis was also performed to gain compositional information through the depth profile of the oxide formed. Six line scans were completed on each sample, with one scan covering the adjacent substrate region also. The line scans were made perpendicular to the alloy surface, starting in the base alloy then going through the oxide and finishing in the resin. Each line scan was run for 20 minutes.
4.1. Materials Characterisation
Table 4.1 shows the quantitative EDX results for the four alloys examined in this research programme. Also included is the composition of the super 304H samples which had a shot peened inner bore, demonstrating that the two alloy samples were of the same nominal composition. There is a significant difference in the Cr content when comparing the two steel types, i.e. the martensitic steels (T91 and T92) with the austenitic steels (super 304H and 347H FG). Some minor compositional differences can be seen between the martensitic steels and similarly for the austenitic steels. The main difference between the super 304H and the 347H FG is the copper content, added for creep strength, and niobium content, which is added to 347H FG for creep strength as well. The niobium in the super 304H is used for solid solution strengthening.
Table 4.1. The compositions of alloys tested in wt-%, determined by EDX.
Alloy (wt-%) Si V Cr Mn Fe Ni Nb Mo W Cu T91 post service 0.3 0.3 9.3 0.4 89.6 0.1 - - - - T92 0.1 0.3 9.3 0.7 86.8 0.3 - 0.5 2.0 - Super 304H 0.2 - 19.0 1.0 68.1 8.6 0.5 - - 2.6 Super 304H shot peened 0.3 - 19.3 1.0 67.5 8.5 0.7 - - 2.8 347H FG 0.5 - 19.2 1.8 66.4 10.8 1.4 - - -
The appearance of the inner surfaces of the tubes in the as-received condition is shown in Figure 4.1. All inner surfaces are shiny except the T92 sample which is covered by a dark oxide (Fig 4.1a.).
Figure 4.1. Optical macrographs of the inner surfaces of the as-received tubes, a.) T92 with pre-existing dark oxide, b.) super 304H, c.) shot peened super 304H which is shinier than the standard super 304H surface, and d.) 347H FG.
Figure 4.2 shows electron micrographs of the inner surfaces of the three austenitic stainless steel tubes. The super 304H and 347H FG have a very similar rough surface finish, the inside of the tubes are almost identical. This is likely due to a pickling process in manufacture. However, super 304H had intermittent small grooves running along the length of the tube. The difference between the super 304H and shot peened super 304H inner surfaces is very apparent, the later is much smoother without grooves and the granular roughness. The shot peened surface also has overlapping dimples as seen in Fig 4.2b.
Figure 4.2. Secondary electron micrographs of the as received inner surfaces of a.) super 304H b.) shot peened super 304H and c.) 347H FG. The surfaces of the super 304H and the 347H FG look similar.
4.1.2. Grain Structure As-Received
Cross-sectional optical micrographs of the etched steels in the as-received condition are shown in Figures 4.3 to 4.6. The etch with Viella’s solution clearly shows the uniform equiaxed grain structure of the T92 alloy in Figure 4.3. The surface was uneven and covered in a continuous uniform oxide.
Figure 4.3. Optical micrographs of the as received T92 cross sectioned and etched in Viella’s solution showing grain boundaries and the martensitic structure within.
The 347H FG was electrolytically etched in 10% oxalic acid at 5V to reveal the twinned austenitic equiaxed grain structure shown in Figure 4.4. This was uniform throughout the sample up to the sample edge, which was uneven and did not already have an as received oxide formed.
Figure 4.4. Optical micrographs of the as received 347H FG electrolytically etched in 10% oxalic at 5V acid showing austenitic grain structure and boundaries.
The super 304H was etched electrolytically to reveal the twinned austenitic equiaxed grain structure shown in Figure 4.5. The inner surface was very uneven and contained no as received oxide.
Figure 4.5. Optical micrographs of the as received super 304H electrolytically etched in 10% oxalic acid at 5V revealing austenitic grain structure.
Comparison of Figure 4.6 to Figure 4.5 shows that the effect of shot peening the super 304H penetrates to approximately 30µm, where the grain boundary density has increased. The surface is much smoother with intermittent overlapping dimples as seen on the surface images.
Figure 4.6. Optical micrographs of the as-received shot peened super 304H electrolytically etched in 10% oxalic acid at 5V showing the austenitic grain structure and compressed surface region.
4.2. Oxidation in Air
4.2.1. Mass Change Results
All three austenitic steels follow a similar gradual mass gain when exposed in air at 600oC, Figure 4.7. At 500 hours the mass gain appears to level out and even slightly decrease with types 304H and shot peened 304H. The shot peened super 304H consistently shows the least mass gain. At this temperature the 347H FG appears to show the greatest mass gain and worse performance (in terms of oxidation resistance) than the super 304H samples, Figure 4.8. This is not the case at 650 and 700oC where they appear to be equal. The martensitic T92 steel did not show any mass gain, Figure 4.7, and showed an increasing mass loss over time with substantial mass loss (-1.45 mgcm-2) after 1000 hours. This significant mass loss represents large scale spallation of the non abraded side on the inner surface of the tube.
Figure 4.7. A graph showing the mass change per unit area for selected steels at varying durations at 600oC.
Figure 4.8. A graph showing the mass change per unit area for just the austenitic stainless steels at varying durations at 600oC.
Figure 4.9 shows selected samples after 600oC air exposure. The T92 sample shows widespread oxidation on both abraded and non-abraded sides, however, much of the abraded side still remained shiny. At 1000 hours T92 shows severe cracking and spallation on the non-abraded (left) side after cooling. No observable spallation was seen on the austenitic steels, just a change from shiny to a dull appearance from oxidation. However, the shot peened super 304H was the only steel to still remain shiny in appearance.
a.) 1000h 250h b.) 500h d.) 1000h c.) e.) 500h 1000h f.) g.) h.) 500h 1000h
Figure 4.9. Optical macrographs showing the following sectioned samples after being exposed to 600oC a.) T92, 250h, b.) T92, 1000h, c.) super 304H, 500h, d.) super 304H, 1000h, e.) super 304H shot peened, 500h, f.) super 304H shot peened, 1000h, g.) 347H FG, 500h, h.) 347H FG, 1000h.
The mass gain at 650oC for the austenitic steels shows a similar increasing trend to before, and a significant mass loss for the T92 martensitic steel, Figure 4.10. The mass gain of the austenitics again plateausafter 500 hours with the shot peened samples consistently having the smallest mass gain and the standard super 304H having the greatest, Figure 4.11.
Figure 4.10. A graph showing the mass change per unit area for steels at varying durations at 650oC.
Figure 4.11. A graph showing the mass change per unit area for just the austenitic stainless steels at varying durations at 650oC.
The optical macrographs shown in Figure 4.12 illustrate the oxidised inner surfaces of the samples after exposure to 650oC. Both T92 samples show large scale cracking and spallation on the non abraded (left) side after cooling. After 1000 hours the T92 abraded side now has a dull appearance, indicating a thicker oxide growing. The austenitic steels show a dark/dull appearance due to oxide formation with no observable spallation. The 347H FG after 500 hours had a slightly uneven contrast appearance compared to the other samples.
a.) 100h b.) 1000h c.) 1000h 500h d.) 500h 1000h e.) f.) 500h h.) 1000h g.)
Figure 4.12. Optical macrographs showing the following sectioned samples after being exposed to 650oC a.) T92, 100h, b.) T92, 1000h, c.) super 304H, 500h, d.) super 304H, 1000h, e.) super 304H shot peened, 500h, f.) super 304H shot peened, 1000h, g.) 347H FG, 500h, h.) 347H FG, 1000h.
At 700oC the mass gain of the austenitic steels was similar to before. Mass gain was the least for the shot peened super 304H, with the austenitics appearing to level off after 500 hours (Figure 4.13). However, the T92 showed a different trend in mass change to the lower temperatures. It showed a mass loss after 100 hours but after the longer durations showed a considerable mass gain much greater than that of the austenitic steels (Figure 4.14).
Figure 4.13. A graph showing mass change per unit area for just the austenitic stainless steels at varying durations at 700oC.
Figure 4.14. A graph showing mass change per unit area for selected steels at varying durations at 700oC.
The T92 samples after cooling from 700oC show no large scale cracking or spalling of oxide scale on either the non abraded (left) or abraded (right) side, Figure 4.15. This is consistent with the greater mass gain. However, at 700oC the abraded side is no longer shiny and was dull/dark in appearance. The oxide on the non abraded side has remained adherent to the substrate on cooling. The austenitic stainless steels all appear darker after the oxide has formed.
500h a.) 1000h b.) 500h 1000h c.) d.) e.) 500h f.) 1000h 500h 1000h g.) h.)
Figure 4.15. Optical macrographs showing the following sectioned samples after being exposed to 700oC a.) T92, 500h, b.) T92, 1000h, c.) super 304H, 500h, d.) super 304H, 1000h, e.) super 304H shot peened, 500h, f.) super 304H shot peened, 1000h, g.) 347H FG, 500h, h.) 347H FG, 1000h.
4.2.2. Overall Thickness Analysis
The average inner surface oxide thickness measurements were taken for each sample. The oxides forming on the samples were initially nodular and discontinuous resulting in high standard deviations for the initial duration thickness measurements (see Appendix A.2). All oxide growth was initailly fast and then slowed down after 100 hours. The oxide formed on the shot peened super 304H samples was not thick enough to be measured on many of the samples especially at lower temperatures and shorter durations. The oxide growth on the T92 samples could also not be measured due to mass spallation on the non abraded side on cooling, and the relatively thin oxide grown on the abraded side.
At 600oC there was a rapid initial growth in oxide thickness, which then slows down for the super 304H and 347H FG samples. Both samples showed a slight decrease in growth of the oxide after 250 hours (Figure 4.16). The oxide formed on the 347H FG inner surface was consistently thicker than that formed on the super 304H.
Figure 4.16. Graph showing the average oxide growth for durations up to 1000h at 600oC. Measurements for the shot peened samples could not be taken due to their minute size.
At 650oC the super 304H and 347H FG samples showed a slow growth in oxide thickness after initial rapid growth (after 100h); see Figure 4.17. At this temperature however, the super 304H samples appear to have a thicker oxide growing on them than the 347H FG which is opposite behaviour to these samples at 600oC. The oxide forming on the shot peened sample after 1000 hours was thin but measurable.
Figure 4.17. Graph showing the oxide growth for durations up to 1000h at 650oC. Measurements for the shot peened samples could not be taken due to their minute size (except at 1000h).
The samples at 700oC also showed a slow increase in thickness after an initial rapid growth with the oxides formed on the super 304H being consistently thicker than the oxides on the 347H FG, Figure 4.18. The oxides formed on the shot peened super 304H were measurable after 500 hours, however no increase in oxide thickness was seen.
Figure 4.18. Graph showing the oxide growth for durations up to 1000h at 700oC. Measurements for the shot peened samples could not be taken due to their minute size (except at 500h and 1000h).
Figure 4.19 shows cross section examples of the oxide formed on the T92 non abraded side after 100 and 1000 hours at each temperature. At 600oC the T92 non abraded side spalled severely after each duration. Image a.) shows the cross section through a sample oxidised for 100 hours which has remained adherent. The oxide is approximately 70µm thick. Whereas image b.) at 1000h shows a spallated region showing only an inner subscale remaining adherent, of approximately 5µm thick. This remaining adherent inner oxide is also present in image d.) and e.) but is not as obvious in f). The oxide has remained adherent in the cross section area at 650oC after 100h in image c.); however, there is extensive cracking between the inner and outer oxide layers, which will increase the risk of spallation. The oxide consistently spalled on cooling from 600oC and 650oC but remained adherent on most of the T92 700oC samples, including after 1000h as seen in image f.). Here there are small cracks starting to form between the substrate and oxide. The thick oxide remaining on T92 samples is porous and therefore less protective than a dense thinner oxide.
Figure 4.19. Back scattered electron images of the T92 oxides formed on the non abraded side at 600oC after 100h and 1000h (a and b), at 650oC after 100h and 1000h (c and d), and at 700oC after 100h and 1000h (e and f).
Figure 4.20 shows the cross sectional micrographs of oxide formed on the super 304H samples after 100 and 1000 hours at each temperature. It is apparent that after 100 hours the oxide forming in nodular and discontinuous in morphology (a., c., e.). At higher temperatures the oxide nodules are larger and starting to join together. For longer durations such as 1000 hours, the oxide continues to grow both vertically and laterally, so that the intermittent nodules coalesce to form a morecontinuous, uniform oxide layer as seen in images b.) d.) and f.).
Figure 4.20. Back scattered electron images of the super 304H oxides formed at 600oC after 100h and 1000h (a and b), at 650oC after 100h and 1000h (c and d), and at 700oC after 100h and 1000h (e and f).
The cross sectional analysis of etched super 304H samples revealed the early nodular oxide growth morphology, Figure 4.21. The nodules appear to grow on the individual grains, with the edges of the nodules associated with the grain boundaries in the substrate. At grain boundaries on the substrate surface no visible oxides are apparent at the magnifications and resolution of the SEMs used.
Figure 4.21. Cross-sectional back scattered electron images of super 304H oxidised at 600oC for 100h and electrolytically etched in 10% oxalic acid showing nodular oxide growth in between grain boundaries with no obvious oxides at the grain boundaries.
EDX analysis, Figure 4.22 and Table 4.2, shows that these initial nodules are Fe-rich oxides with a suggested FeO composition containing minimal chromium. The standard deviations for the elements with smaller concentrations are large due to EDX sampling elements from the rest of the alloy. This has been observed for small element concentrations throughout EDX analysis.
Figure 4.22. The site of interest for the EDX point scans completed on the oxide nodules formed on the super 304H after 100h at 600oC.
Table 4.2. The average EDX point scan results of the super 304H oxide after 100h at 600oC in atomic %.
O Si Cr Mn Fe Ni Cu
Oxide 47.8 ±2.4 - 2.7 ±3.0 - 49.0 ±2.5 0.5 ±0.5 0.6 ±1.3
The images in Figure 4.23 show cross sectional micrographs of the shot peened super 304H samples after 100 and 1000 hours at each temperature. The smooth shot peened surfaces show little visible oxide forming after most durations. The majority of the cross sectioned samples show a crack to have formed between the resin and the sample surface which was filled with polishing debris and possibly broken oxide. However, at higher temperatures after longer durations visible oxide was recorded (Figure 4.23, f.). This oxide was up to 1µm in thickness and partially delaminated.
Figure 4.23. Back scattered electron images of the shot peened super 304H oxides formed at 600oC after 100h and 1000h (a and b), at 650oC after 100h and 1000h (c and d), and at 700oC after 100h and 1000h (e and f).
At certain points along the inner surface of the shot peened super 304H tube, indents into the alloy surface were observed, which were full of oxide. Figure 4.24, shows examples of these small crevices or cracks in the surface which experienced large oxide growth which is not consistent with the rest of the smooth shot peened surface. These examples clearly demonstrate the effect of shot peeing on oxidation and the limitations of the process on some features of the tubes.
Figure 4.24. Back scattered electron images of the shot peened super 304H showing examples of regions on the surface where the shot peening process has not reached some cracks and crevices showing a pronounced increase in oxidation. Image a.) from exposure to 700oC after 250h and b.) 650oC after 1000h.
Figure 4.25 shows the morphology of the oxide formed on the 347H FG samples after 100 and 1000 hours at each temperature. The thickness and geometry of the oxide is similar to that of the oxides formed on the super 304H samples, however the lateral growth of the nodules formed on the 347H FG appears to occur earlier. After 1000 hours the oxide on the 347H FG becomes more uniform in thickness as it grows. These samples did not suggest a thicker oxide with increasing temperature.
Figure 4.25. Back scattered electron images of the 347H FG oxides formed at 600oC after 100h and 1000h (a and b), at 650oC after 100h and 1000h (c and d), and at 700oC after 100h and 1000h (e and f) showing a more uniform oxide.